9. Real Steel
9.1 Some General Remarks
9.1.1 Things Get Complicated
|Properties and Microstructure Reconsidered|
|So far I have mostly looked at an
ideal iron - carbon alloy, called plain
carbon steel, with just an occasional glance of what else might be in
there. This is not realistic. In ancient steel, there is always something else in there - essentially the
more prominent elements of the periodic table in some form or other and inclusions of slag particles, charcoal,
"pebbles", and whatever else was around. Whatever is in there got
inside by circumstances and certainly not
by intention. Aristotle, after all, had proclaimed that
especially pure iron, so why should you add something?
Even if you, the ancient smith who had fortunately never heard of Aristotle, dunked your red-hot iron in all kinds of revolting stuff including goose shit, you didn't do it in order to get some element inside the steel crystal lattice. You believed in the working of some magic that somehow relates to goose shit or whatever, or you simply did it because somebody (your master) had told you that this is what one does. Just think of all the revolting stuff people eat just because somebody (typically parents) told them that this is what one does, and you see how powerful tradition can be. My wife (from NYC), for example, eats slime that's is still alive! inside some closed (for good reasons!) nacre shell!
Times have changed. When we make modern steel, we add all kinds of alloying elements intentionally. But mostly we also have some stuff in there that we do not care about. The only question is if we know that some unintentional stuff is in there, and how we make sure that we can tolerate it. We need to distinguish a bit more closely between the various things our iron / steel might contain and define a few terms:
|The periodic table contains about 90
elements that you can find out there, if mostly in disguise, i.e. tied up in
some compound. You can also just buy most of them, something that is much
easier to do. Some elements are very rare and thus not likely to be
unintentionally incorporated in your steel. That is one reason why many of
those 90 elements are only found in very low concentrations in your steel,
ppm or much lower.
You need sophisticated equipment to detect them.
It is very likely that a very low concentration of something does not influence the properties of your steel very much - but you never know for sure. Boron (B), for example, will be felt at concentrations as low as 0.0003 % (3 ppm).
|But many elements are ubiquitous
enough and thus might make it into your steel. Assuming that we always have
some carbon around, we have, expanding on
the above a bit, the following basic possibilities:
| As you see, steel science is
difficult. Very difficult. What we learn from all of the above is that just
knowing the concentration of some element doesn't tell you how it might change
properties. And I'm meaning all relevant
properties, not just the basic "strength" stuff that I mostly
discussed so far. And whatever it does in principle will very much depend on
processing. And on what else is in there. And on the temperature and the
Nowadays we may know the exact composition of a steel down to trace elements in the ppm or even ppb range - but that does not tell us all that much about its properties. The properties, as you know by now, depend on the microstructure, which depends on the compositions and the processing, or everything you or somebody else ever did to your steel.
|To make things even more complicated
we must now also consider steels without
carbon or more properly, steels with very low carbon concentrations.
The link will tell you far more about that than you ever wanted to know. These
"designer steels" are always
modern steels and their number and market share is rapidly growing. Don't mix
that up with old-fashioned wrought iron. It
is low in carbon, yes, - but it is not steel!
You can already appreciate that with only a little carbon you cannot produce much cementite. Hardness thus must come from something else. I will come to that.
|Of course, over the last 150 years or so, when something akin to steel science was born and thrived, a lot of data have been collected and refined into knowledge and rules. But that only helps to some extent, because there is almost no rule without exception. Sulfur in steel is always bad? Yes, but there are some steels where sulfur (S) is added intentionally because it makes machining easier. Even evil phosphorous is used in modern so-called "weathering steel" and some others. Another example is oxygen. It is decisive for making your steel. You blow it through your molten raw stuff in order to take out you whatever you don't want, but you typically don't want it in the solidified product1).|
|So, once more, steel science and
engineering is difficult. Very difficult. Thank God! It gives us scientists and
engineers something to do for making a living. If systems are very complex,
then there is also a lot you can do.
Look at modern alloy steel; iron with alloy elements that we put in there intentionally. I, a modern steelmaking scientist have an incredibly large selection of alloying elements and processes up my sleeve, from which I can choose. That's why there are thousands of different iron alloys out there today, all of them we call "steel". And that's why there will be many more to come, just wait. The parameter space involved is still largely unexplored. In contrast, you, the ancient smith and steelmaker (almost the same thing) had only very limited options. Worse, you had not much leeway in exercising these options either.
option was to choose among the few kinds of steel available two
thousand or three thousand years ago.
Your third option was which God you prayed and made sacrifices to. It might have helped your spiritual well being but did very little towards improving your steel.
|At this point you must become aware
once more that what I have summarily called slag
inclusions are objects of prime importance for all ancient smiths
making iron and steel objects including sword blades, from all steel other than
wootz steel. Inclusions are the major reason for all this folding and
hammer-welding; I'll get to that.
But let's assume that we know that it is the microstructure, including slag inclusions, that determines the properties in the end. Let's think about this for a minute. Do we (I include myself) really know how the properties of steel depend on the microstructure?
|Let's say we know the exact composition of a
steel and its microstructure. That allows
you and me (in principle) to make some educated comments or guesses about its
hardness and ductility, allright. But how about the following
Then you repeat most of the list but for some temperature other than room temperature. Is fatigue more pronounced at high temperatures?
|The answers to the many questions hinted at above
must be hiding in the microstructure. There simply is nothing else. My
colleagues and I (mostly my colleagues, to be honest) indeed do know a lot
about how all these properties depend on the composition and the
microstructure. Not yet all there is to
know, but a lot. I give you a taste treat in two advanced modules about
creep and fatigue.
I will not say much about corrosion - yet. It's too painful, see below. Not only for the owner of fine steel products but also for Materials Scientists. While we do know a lot about corrosion, it's not nearly as much as we would like to know.
|Some smith around - roughly - 500 AD
made a complex pattern-welded sword from two kinds of steel. One of these
steels was phosphoric steel (I'll get to that shortly), the other one carbon
steel. Look at what you get after only a millennium and a half! The carbon
steel is almost gone whereas the phosphoric steel was rather corrosion
resistant under the conditions encountered.
And that is even a well-preserved artifact. Most of those swords, originally looking like that, are now only a vague orange colored spot in the earth.
|Of course there are a lot of basic rules about properties and microstructure. Most of them were found empirically and explained later, if at all. I will give you one important rule as example:|
| Tough luck! Our main ingredients for
increasing hardness cause severe problems regarding other properties. So we
need to do something about that by alloying the right elements besides carbon.
That's essentially why we do extensive alloying. As far as only hardness is
concerned, just working with (clean) iron and carbon would already do a good
The good news thus is: With proper alloying you can cure some problems of your steel.
|However, there is still no such thing
as a free lunch.
The bad news is: There is no super steel that gets only good grades with respect to all the 20 plus properties of interest to you when you consider a product. One size doesn't fit all.
To some extent this is clear. Super steels cannot exist because quite often some requirements on your list are contradictions in terms. You just cannot have a steel that is easy to press into some shape (so it must have a low yield stress) and very hard (requiring high yield stress) at the same time. It's just like demanding a round square, esoteric science or theo logy.
Good grades in all non-contradicting properties are not possible either; in particular if one of those properties is called "costs count", i.e. if the great cost issue raises its ugly head.
|The message is clear: you must compromise! You might be looking all your
life for that gorgeous person with a Noble prize in physics, a lot of money, a
friendly and honest disposition, and so on, but you are most likely better off
to compromise when looking for a partner (especially if you are a physicist).
You might be looking all your life for that supersteel either. Going for the best compromise is smarter.
|That's why there are far more than 1000 types of steel out there that you can buy. In a few years from now there will be even new types - steel science and engineering is still far away from having made everything that has some value for somebody. Development of new steel types is more and more based on solid science including a lot of computing. That does not preclude that on occasion some "tinker" comes up with a big surprise.|
|You realize of course that we are now
deeply in non-crystalline organic waste, to say it politely. How do we make a
catalogue listing that many types of steel in a systematic fashion? How do we
It's like categorizing the many different types of wine or living beings. "Red, white, rosé", or "animals, plants, fungus" comes to mind and gives an easy start - and some trouble. Under which wine heading would you list champagne or "Schillerwein" a German specialty where you mix red and white grapes? Are viruses living beings and if so, which heading covers them?
The real trouble, of course, starts after the first level of the system. The next level of listing wines, for example, may contain identifiers like grape type (e.g. Lemberger, Pinot Noir, Zinfandel, Primitivo, ..) or region: Württemberg, Napa valley, California, Bordeaux, Rioja, ...). It's not overly helpful. I bet you don't know what a Lemberger grape is (my preferred variety) or that Zinfandel and Primitivo are just two different names (USA and Italy, resp.) for the same grape. Giving the sugar content (or words for it like "dry" or semi-dry") and so on comes next, plus lots of entertaining descriptions ("steely with a hint of flint"). And you know what: It doesn't tell you much about how some wine will agree with you if you don't have extensive prior experience with wines and the classification system.
|Historically, wine was only categorized by its origin. The same is true for steel. Where it was made (or who made it) told you how it was made and what kinds of properties and quality to expect. "Sheffield steel" or "Krupp Stahl" said it all. Some areas or producers just produced better wine or steel than others, and nobody knew exactly why this was the case.|
|Categorizing steels is almost as bad as listing wines. I won't even attempt it here.||
|This Hyperscript, however, claims to encompass
everything remotely interesting to swords, and that must include some way to
classify steels. I therefore give you the basics about categorizing steels in a
It is basic and not advanced because is contains absolutely nothing that is difficult. It just is awful, illogical, wretched and complicated - even so no politicians and lawyers were involved.
|Getting Closer to Real Steel|
|In a general and somewhat trivial way
we distinguish between the unwanted evil impurities called dirt, and the wanted good ones that we then call
alloy elements. There are thus two reasons
why you have foreign atoms in your iron or steel:
|The first point, of course, relates to iron and steel making for the first 3.500 years or so, the second point to the way we do it for the last 100 years or so.|
|I will get back to modern steel making, but for now let's look at the old-fashioned way. Both kinds of elements, the badies and the goodies, then come almost exclusively from the ingredients used in the making of the steel, including the ingredients used for optimizing slag. I'll get to slag in the fullness of time.|
|In ancient times you stuffed unclean
ore and unclean charcoal into your smelting furnace. You had no choice, you
simply didn't know better. You might have had an idea that cleaner is better,
though. Remember? All that was known about the "theory" of steel is
that Aristotle had
proclaimed around 350 BC that steel was
So you may even have treated your ore before you used it, removing some of the unwanted stuff, but nonetheless your ingredients were never very clean. In our modern times we still stuff unclean ore and "coke" into our huge blast furnaces. Not because we couldn't make clean ore and carbon but because it's impossible to get clean carbon and pure iron ores in huge quantities for very little money. Coke in this case means rather clean carbon and is not something you drink or stuff up your nose. I'll get to coke in the fullness of time, too.
|Whatever happens inside your blast furnace (and that's a rather complex story we are going to tackle in the next chapter), you cannot reasonably expect that pure iron will come out. Nevertheless, our forebears did produce admiringly clean wrought iron in their primitive "bloomery" furnaces. They could do that because they made very clever use of the iron-carbon phase diagram - without having the slightest notion of what that might be. Their stuff always contained slag inclusions, however.|
|By the way, the silicon (Si) production of today follows the same basic ideas we use for making iron. You throw dirty silicon "ore" (actually silicon oxide or silica (SiO2), otherwise known as quartz sand) and dirty coal / coke into a furnace. You even add some more dirt in the form of (special) wood chips because that makes the product better - just like the special plants put in the crucible when making wootz steel. The only difference to iron making is that you don't set the mix on fire. You run some heavy electric current through it. It's necessary for some particular reason but the effect is the same. Things get rather hot.|
|What you get is - surprise - dirty
silicon. There is
a lot of dirty silicon (also called "metallurgical grade silicon")
made every year; well above one million metric tons. Most of this metallurgical
grade silicon goes - you guessed it - into steel or aluminum as
element. An amazingly large part is also used to make
silicone, a polymer that has
many uses, some of them associated with outstanding properties of people like
By the way (once more), you noted (I hope) that silicon, silicone, and silica are about as different as romanic, romantic, and Rome, or "Smelting", "melting" and "gelding". Unfortunately this is not always known to journalists, translators or museum people.
A small part of the metallurgical grade silicon, about 25.000 tons per year or 2 % of the total, is converted to the ultra-clean and quite expensive single-crystal silicon that ends up in computer chips, solar cells, or micro-mechanical devices like the "heart" of your beamer or the movement sensors in your i-phone.
|Only a small part of the total iron / steel production of old ended up in a superior sword. The product then is expensive and so on, but also demonstrates the top technology of the time. That's what motivated my (amateur) interest in swords, remember?|
|It also motivates my (professional) interest in solar cells. While we can make an enormous number of computer chips from one ton of ultra-clean silicon, one ton won't get us very far if we want to make square miles of solar cells with silicon. That's why there are large efforts under way to learn how one could make good solar cells with dirty||
|and cheap "metallurgical grade" silicon. It will be rather exciting for the initiated to watch if the silicon guys can do what the steel guys managed to do 2000 years earlier by cunning, and about 150 years ago by evolving into Materials Scientists and Engineers. They either learned how to live with dirt or how to remove it cheaply.|
| I'm absolutely sure we
will succeed with silicon, too. We are already at the "break even"
point now (2012), i.e. producing your electricity with solar cells cost just as
much as in the old-fashioned way. That can be roughly compared to the point in
time when mass-produced steel had its "break-even" with the
dominating cast iron. Just wait an other 20 years and solar energy will be far
cheaper than running power plants with coal, oil, or gas.
Yes, you are right - the sun doesn't shine at night; in my country quite frequently we do not even see her during the day. I know that. All I have to say is: trust your scientists and engineers to find a solution. Don't trust your bankers, oil companies, power plant owners and related politicians to find a solution. And keep the latter from hassling the former.
In particular, do kick your economist in the rear when he tells you that the solution will be to write some numbers on paper (called CO2 emission certificates). I guarantee that they will work just as well as the papers pronouncing fledgling dot.com companies to be more valuable than, let's say, Mercedes; the papers that promised to yield far more then 20 % a year by bundling mortgages yielding around 3 %; or the papers stating that Greece is a healthy economy ready to join the euro. Not to forget, of course, all the papers stating that a crisis that resulted from overspending, can only be overcome by more overspending.
So trust my colleagues and me in particular. If it makes you feel better, you could send me large amounts of money and I will send you a paper stating in many fancy words that the energy crisis and the financial crisis is now over for you. Don't miss this opportunity! I will serve only the first 1000 applicants, the rest will have to live with both crisis' forever after.
|1)||Dianzhong Li, Xing-Qiu Chen, Paixian Fu, Xiaoping Ma, Hongwei Liu, Yun Chen, Yanfei Cao, Yikun Luan & Yiyi Li, in the article "Inclusion flotation-driven channel segregation in solidifying steels", published in: Nature Communications 5, Article number: 5572 in Novemebr 2015, report the observation that "Channel segregation, which is featured by the strip-like shape with compositional variation in cast materials due to density contrast-induced flow during solidification, frequently causes the severe destruction of homogeneity and some fatal damage" is caused by oxygen precipitation and occurs for oxyen concentrations above 0.001 wt%. "This study uncovers the mystery of oxygen in steels, extends the classical macro-segregation theory and highlights a significant technological breakthrough to control macrosegregation" is claimed by the authors.|
© H. Föll (Iron, Steel and Swords script)